Tensile Strength,Yield 1022 MPa 148000 psi Hardened 1800°F,Tempered 550°F Tensile Strength,Yield 1026 MPa 149000 psi Hardened 1800°F,Tempered 600°F Tensile Strength,Yield 1076 MPa 156000 psi Hardened 1800°F,Tempered 400°F Tensile Strength,Yield 290 MPa 42100 psi 0.2% offset,Annealed Tensile Strength,Yield 589 MPa 85400 psi
410.410 stainless is a corrosion and heat resistant 12% chromium steel.It is the most widely used of the hardenable stainless steels.Heat treated 410 has mechanical properties comparable to the engineering alloy steel AISI 4130,coupled with the additional benefit of good corrosion resistance.410 is highly resistant to atmospheric corrosion.
410 is a basic straight chromium high hardenability martensitic stainless steel with good strength and fairly good corrosion resistance as generally supplied hardened and tempered in the tensile range 700 - 850 Mpa (condition R) Brinell range 201 - 255.Characterised by good corrosion resistance in mild atmospheric industrial and domestic environments coupled with good strength and excellent410 Stainless Datasheet - United Performance MetalsType 410 is hardenable,straight-chromium stainless steels which combine superior wear resistance of high carbon alloys with the excellent corrosion resistance of chromium stainless steels.Oil quenching these alloys from temperatures between 1800°F to 1950°F (982-1066°C) produces the highest strength410 Stainless Steel Annealed - Bergsen MetalThe mechanical properties of 410 annealed stainless steel at a mean temperature of 68º F (20º C) include Yield Strength 0.2% Offset 42,000 psi (290 MPa) Ultimate Tensile Strength 74,000 psi (510 MPa) Elongation in 2 in.34%; Hardness 96 Rb max Fabrication Data of 410 Stainless Steel Annealed
410 is the basic,general purpose,hardenable martensitic stainless steel.It is used for highly stressed parts with good corrosion resistance and strength.410 Stainless Steel Bar - Annealed,Edge Conditioned,Hot Rolled True Bar TW Metals410 Stainless Steel McMaster-CarrTight-Tolerance Wear-Resistant 410 Stainless Steel.Yield Strength 30,000 psi.Hardness Rockwell B95 (Medium) Heat Treatment Annealed (Softened) Heat Treatable Yes.Max.Hardness After Heat Treatment Rockwell C30.Specifications Met ASTM A240.Precision ground on the top and bottom to a tight tolerance,these sheets and bars are also 410 Stainless Steel Properties KVA StainlessAISI Type 410 is a martensitic stainless steel that provides high strength and hardness with moderate corrosion resistance.A wide range of properties can be developed with different heat treatments,with ultimate tensile strengths ranging from 500 to 1400 MPa.It is magnetic in both the annealed and hardened conditions.
Grade 410 stainless steel is a hardenable,martensitic stainless steel that features a minimum addition of 11.5% chromium.This addition of chromium provides a significant increase in corrosion resistance in mildly corrosive environments where high strength and moderate heat resistance are required.It adequately resists sulfuric acid,nitric acid,and weak acetic acid.410 Stainless Steel Technical Data Sheet - metal shimsType 410 is a hardenable,straight chromium stainless steel which combines superior wear resistance of high carbon alloys with the excellent corrosion resistance of chromium stainless steels.Oil quenching these alloys from temperatures between 1800°F to 1950°F (982 to 1066° C) produces the highest strength and/or wear resistance as well as 410 Stainless Steel UNS S41000 Strip,Foil Wire Type 410 is a martensitic stainless steel that provides good corrosion resistance plus high strength and hardness.It is magnetic in both the annealed and hardened conditions.A wide range of properties can be achieved with different heat treatments.
Jun 21,2020·Type 410 steel is the basic general-purpose steel used for steam valves,tray valves,pump shafts,turbine blades,bolts and miscellaneous parts that require corrosion resistance and moderate strength up to 540°C (1000°F).SS 410 Equivalent MaterialASTM A276 410 Round BarSS 410 Round Bar410 BrightASTM A276 410 Round Bar Definition.Prosaic Steel and Alloys,are Recognized as the Prominent Manufacturer,Exporter and Supplier of a broad assortment of ASTM A276 347 Round Bar.The offered ASTM A276 347 Round Bar is designed with utmost precision in conformity with the international quality standards..ASTM A276 347 Round Bar can be categorically said that steel bars are one of the core ASTM A276 Type 410 - FERROBENDASTM A276 Type 410 is a material grade specification for cold-finished or hot-finished bars in 410 stainless steel,available in form of rounds,square,hexagons and other hot rolled extruded shapes.Ferrobend offers 410 bars,shafts,angle,channel,beam profiles,bolts,studs,screws,nuts,threaded rods,pins and other bar stock components to astm a276 type 410 specification.
For maximum hardness and strength,a hardening heat treatment is necessary.The stainless steel alloys shown in the table above were heated as sheet samples for 60 minutes per inch of thickness at 1800°F (982°C) for Type ATI 410 and at 1900°F (1038°C)Alloy 410 Martensitic Stainless Steel Plate - Sandmeyer SteelAlloy 410 stainless steel plate is the general purpose 12% chromium martensitic stainless steel that can be heat treated to obtain a wide range of mechanical properties.410 stainless steel plate possesses high strength and hardness coupled with good corrosion resistance.Alloy 410 stainless steel plate is ductile and can be formed.Composition Fe/<.15C/11.5-13.5Cr/<1Ni/<1Mn/<1Si/<.04P/<.03SMaterial Stainless Steel - Grade 410 (UNS S41000)PROPERTYMINIMUM VALUE (S.I.)MAXIMUM VALUE (S.I.)UNITS (S.I.)Atomic Volume (average)0.00710.0074m3/kmolDensity7.657.85Mg/m3Energy Content84102MJ/kgBulk Modulus140163GPa 28 rows on azom410 STAINLESS STEELAK Steel Type 410 is a martensitic stainless steel that provides excellent corrosion resistance plus high strength and hardness.It is magnetic in both the annealed and hardened conditions.A wide range of properties can be developed with different heat treatments.Applications requiring moderate corrosion resistance and high mechanical properties are ideal for this alloy.
T-410,T-410S.12% Chromium hardenable martensitic stainless steel.T-410 is the basic chromium grade in the '400' series.It can be treated by conventional means to develop high strength properties with good ductility.In fact,it is in the heat treated condition that T-410 develops its maximum corrosion resistance,particularly when ground File Size 100KBPage Count 6HIGH-TEMPERATURE CHARACTERISTICS OF STAINLESSthe strength ranges being considered.As shown,the stainless steels have a higher hot strength than low-carbon unalloyed steel,with the austenitic (300 Series) grades displaying considerably higher strengths than the martensitic or ferritic (400 Series) grades.TheFile Size 1MBPage Count 3Types 410,420,425 Mod,and 440Athe highest strength and/or wear resistance as well as corrosion resistance.A range of as-quenched hardnesses is achieved in these alloys by varying the carbon level from .15% maximum in Type 410 to .60-.75% in Type 440A.These alloys are used where strength,hardness,and/ or wear resistance must be combined with corrosion resistance.APPLICATIONS
Grade B6 is a heat-treated 12% chromium-ferritic magnetic 410 stainless steel with minimum tensile strength requirement of 110 ksi and yield 85 ksi.ASTM A193 specification covers requirements for chemical composition,mechanical properties,hardness,heat-treatment and recommended nuts-washers for Grade B6 Fasteners.File Size 456KBPage Count 2Stainless Steel - Grade 410 (UNS S41000)Topics CoveredIntroductionKey PropertiesCompositionMechanical PropertiesPhysical PropertiesGrade Specification ComparisonPossible Alternative GradesCorrosion ResistanceHeat ResistanceHeat TreatmentWeldingMachiningApplicationsGrade 410 stainless steels are general-purpose martensitic stainless steels containing 11.5% chromium,which provide good corrosion resistance properties.However,the corrosion resistance of grade 410 steels can be further enhanced by a series of processes such as hardening,tempering and polishing.Quenching and tempering can harden grade 410 steels.They are generally used for applications involving mild corrosion,heat resistance and high strength.Martensitic stainless steels are fabricatSee more on azomPublished Oct 23,2001410 Stainless Steel,410 SS,Grade 410 - Permanent SteelYield Strength 0.2% offset (KSI) Tensile Strength (KSI) % Elongation (2 Gauge length) Hardness Rockwell 410 Ann 30 min.65 min.20 min.HRB 96File Size 631KBPage Count 47410 Stainless Steel - Penn StainlessAlloy 410 is the basic,general purpose martensitic stainless steel that is used for highly stressed parts and provides good corrosion resistance plus high strength and hardness.Alloy 410 contains a minimum of 11.5% chromium which is just sufficient enough to demonstrate corrosion resistance properties in mild atmospheres,steam,and many mild
May 30,2020·Hardened AISI 410 vs.Hardened AISI 440C.Both hardened AISI 410 and hardened AISI 440C are iron alloys.Both are furnished in the hardened (H) condition.They have a moderately high 94% of their average alloy composition in common.There areMechanical PropertiesProperties Stainless Steel - Grade 410 (UNS S41000)28 rows·410 is the basic martensitic grade stainless steel.They are optimised for high hardness,
yield strength of stainless steel410 stainless steel tensile strengthstainless steel yield strength chart410 stainless steel chemistry410 stainless steel density410 stainless steel hardness410 vs 316 stainless steel410 stainless steel specification12345NextSpecification Sheet Alloy 410 - Sandmeyer SteelYield Strength Ultimate Tensile Elongation 0.2% Offset Strength in 2 in.psi (MPa)psi(MPa) % (max.) 42,000 290 74,000 510 34 96 Rb Corrosion Resistance Alloy 410 is resistant to atmospheric conditions,water and some chemicals.It can be used in environments containing weak or diluted acetic acid,naptha,nitric acid and sulfuric acid.Stainless Steel 410 - Sunny SteelTypical Mechanical Properties- Stainless Steel 410.Material.Tempering Temp °C (°F) 0.2 % Yield Strength (Mpa) Ultimate Tensile Strength (Mpa) % Elongation in 2.% Reduction of Area.Charpy V Notch Impact Strength (J) Hardness Brinell.
Description.Type 410 is a corrosion and heat resistant martensitic stainless steel containing approximately 12% chromium offering a wide range of mechanical properties through heat treatment.This grade offers a moderate level of corrosion resistance and the maximum resistance is obtained by hardening through heat treatment followed by polishing.Stainless Steel Type 410 Tempered Specialty MetalsDescription.Type 410 is a corrosion and heat resistant martensitic stainless steel containing approximately 12% chromium offering a wide range of mechanical properties through heat treatment.This grade offers a moderate level of corrosion resistance and the maximum resistance is obtained by hardening through heat treatment followed by polishing.Stainless steel grade chart - Atlas SteelsATLAS STEELS SPECIALTY STEELS PRODUCT REFERENCE MANUAL SECTION 9 APPENDICES Printed November 2000 Grade UNS No.Mechanical properties specied (Note 4) Common form Treatment Tensile strength MPa (min.) Yield strength (0.2% offset) MPa (min.) Elongation % in 50mm (min.) Hardness (max) (Note 2) Austenitic stainless steels Plate Annealed
Strength  Yield strengtYield strength is the most common property that the designer will need as it is the basis used for most of the rules given in design codes.In European Standards for structural carbon steels (including weathering steel),the primary designation relates to the yield strength,e.g.S355 steel is a structural steel with a specified minimum yield strength of 355 N/mm².Tempering Temperature (°C) Tensile Strength (MPa) Yield Strength 0.2% Proof (MPa) Elongation (% in 50 mm) Hardness Brinell (HB) Annealed *480 min 275 min 16 min - 204 1475 1005 11 400 316 1470 961 18 400 427 1340 920 18.5 405 3 more rows Apr 12 2021Stainless Steel - Grade 410 (UNS S41000)Was this helpful?People also askWhat are the specifications of 410 stainless steel?What are the specifications of 410 stainless steel?GENERAL PROPERTIES Types 410,420,425 Modified,and 440A (see composition on Page 2) are hardenable,straight-chromium stainless steels which combine superior wear resistance of high carbon alloys with the excellent corrosion resistance of chromium stainless steels.Types 410,420,425 Mod,and 440A